High-Mobility Field-Effect Transistors from Large-Area ... · PDF fileHigh-Mobility...
Embed Size (px)
Transcript of High-Mobility Field-Effect Transistors from Large-Area ... · PDF fileHigh-Mobility...
High-Mobility Field-Effect Transistors from Large-Area Solution-Grown Aligned C60 Single CrystalsHanying Li,, Benjamin C-K. Tee, Judy J. Cha, Yi Cui, Jong Won Chung, Sang Yoon Lee,
and Zhenan Bao*,
Department of Chemical Engineering, Department of Electrical Engineering, and Department of Materials Science andEngineering, Stanford University, Stanford, California 94305, United StatesDisplay Device Laboratory, Materials and Device Institute, Samsung Advanced Institute of Technology, Samsung ElectronicsCompany, Ltd., Youngin 446-712, Korea
*S Supporting Information
ABSTRACT: Field-effect transistors based on single crystalsof organic semiconductors have the highest reported chargecarrier mobility among organic materials, demonstrating greatpotential of organic semiconductors for electronic applications.However, single-crystal devices are difficult to fabricate. One ofthe biggest challenges is to prepare dense arrays of singlecrystals over large-area substrates with controlled alignment.Here, we describe a solution processing method to grow largearrays of aligned C60 single crystals. Our well-aligned C60 single-crystal needles and ribbons show electron mobility as high as 11cm2V1s1 (average mobility: 5.2 2.1 cm2V1s1 from needles; 3.0 0.87 cm2V1s1 from ribbons). This observed mobility is8-fold higher than the maximum reported mobility for solution-grown n-channel organic materials (1.5 cm2V1s1) and is 2-fold higher than the highest mobility of any n-channel organic material (6 cm2V1s1). Furthermore, our deposition method isscalable to a 100 mm wafer substrate, with around 50% of the wafer surface covered by aligned crystals. Hence, our methodfacilitates the fabrication of large amounts of high-quality semiconductor crystals for fundamental studies, and with substantialimprovement on the surface coverage of crystals, this method might be suitable for large-area applications based on single crystalsof organic semiconductors.
INTRODUCTIONOrganic field-effect transistors (FETs) are promising forflexible, low-cost, and lightweight electronic applications, suchas complementary circuits,14 displays,5,6 and sensors.711
Organic thin films have been widely used to fabricate FETdevices due to their facile processability in large areas. Thecharge mobility of p-channel organic thin-film FETs hasreached up to 23.2 cm2V1s1.1216 For n-channel organic thin-film FETs, vapor-deposited devices exhibit mobility as high as 6cm2V1s1,17,18 while solution-processed ones have lowermobility of 1 cm2V1s1.2,1921 Organic single crystals, intheory, are ideal charge-transport media, with fewer structuraldefects and thus better electronic performance than the thin-film counterparts.22 Experimentally, single crystals of organicsemiconductors exhibit hole mobility up to 40 cm2V1s1 andelectron mobility as high as 6 cm2V1s1.2233 Although thecharge carrier mobility of single-crystal devices is much higherthan that of thin-film FETs, single-crystal devices are mostlylimited to fundamental charge-transport research becauseindividual devices are usually fabricated manually, and it isdifficult to scale-up for technological applications. In contrast tocontinuous thin-films where devices can be defined anywhere,crystal growth location is stochastic in nature, and yet, positionregistration between crystals and electrodes is crucial to makeelectronic contacts. Therefore, various attempts have been
made to achieve high-throughput controlled placement ofsingle crystals. Crystals can be either selectively grown wherethe electrodes are located26,34,35 or aligned and subsequentlytransferred onto the pattern electrodes.23 In this work, wereport a facile approach to deposit well-aligned C60 singlecrystals on substrates as large as a 100 mm wafer. FETs basedon these crystals exhibit unprecedented electron mobility above10 cm2V1s1.
EXPERIMENTAL SECTIONCrystals were grown in situ on substrates for FETs. Divinyltetrame-thyldisiloxane bis(benzocyclobutene) (BCB, Dow Chemicals) thinlayers were spin coated from a mesitylene (Fluka) solution(VBCB:Vmesitylene = 1: 30) and thermally cross-linked on a hot plate ina N2 glovebox. A C60 (Alfa Aesar) solution (20 L) was dropped ontoa BCB-covered highly doped silicon substrate (1 cm2) with 300 nmSiO2. A piece of silicon wafer (0.4 0.4 cm
2, pinner) was placed onthe substrate to pin the solution droplet (Figure 1). The siliconsubstrate with the droplet was placed on a Teflon slide inside a Petridish (35 10 mm) sealed with parafilm. Crystals formed on thesilicon substrate after the solvent slowly evaporated on a hot plate of30 1 C. Needle-shaped crystals were grown from m-xylene (Sigma-Aldrich) with a C60 concentration ([C60]) of 0.4 mg mL
1, and the
Received: November 6, 2011
XXXX American Chemical Society A dx.doi.org/10.1021/ja210430b | J. Am. Chem.Soc. XXXX, XXX, XXXXXX
solution dried out in 2 h. Ribbon-shaped crystals were from mixedsolvents of m-xylene and carbon tetrachloride (CCl4, Sigma-Aldrich)(VCCl4:Vmxylene = 4:3; [C60] = 0.4 mg mL
1), and the solution dried outin 1 h. The volume ratio (4:3) was chosen as more m-xylene favoredthe growth of needle crystals and more carbon tetrachloride favoreddisk-shaped crystals. The crystals grown at varied volume ratio will bepublished later. For crystallization in a 100 mm wafer scale, 1.5 mL ofsolutions was dropped on a BCB-covered silicon wafer with pinners(0.4 cm wide) placed at 1 cm intervals. The morphology andcrystalline structures were characterized by optical microscopy (OM,Leica, DM4000m), atomic force microscopy (AFM, Digital Instru-ments MMAFM-2), and transmission electron microscopy (TEM, FEITecnai F20, 200 keV for the needles; FEI Titan 80-300, 80 keV for theribbons; 80 keV was necessary for the ribbons to minimize the beamdamage). FETs were constructed in a bottom-gated configuration bydepositing top-contact source and drain electrodes (80 nm Au), withchannel length of 50 m and width of 1 mm. Currentvoltagecharacteristics of the devices were measured in a N2 glovebox using aKeithley 4200-SCS semiconductor parameter analyzer. The measuredcapacitance of the BCB-covered SiO2/Si substrates was 10 nF/cm
2,and this value was used for mobility calculation. For statistics, data ofcrystal heights and electron mobility are presented as mean SD.
RESULTSMany approaches have been used to align organic semi-conductors.36 Among them, zone casting,37 dip coating,38 andsolution sheared deposition39 showed promising results forpreparing aligned crystals with large grains over large areasdirected by (concentration and/or temperature) gradients atthe receding meniscus. Adopting a similar principle ofalignment, we designed a simple droplet-pinned crystallization(DPC) method (Figure 1a) with several advantages over theprevious methods. The operating principle of this approach isas follows: During drying of a droplet of a semiconductorsolution on a substrate, crystals nucleate near the contact lineand grow along the receding direction (toward the center) of
the droplet. Using this method, well-aligned C60 needle andribbon crystals were prepared (Figure 2a,d). We have alsosuccessfully applied this method to other organic semi-conductor materials, such as 6,13-bis(triisopropyl-silylethynyl)pentacene (TIPS-pentacene)40 (Figure S1, Supporting In-formation).Two important requirements need to be satisfied to induce
alignment. First, a high nuclei density (i.e., high solutionconcentration) is required to introduce a mass depletionbetween the nuclei. Only the nuclei with a preferential growthdirection along the droplet receding direction (i.e., masstransport direction) can continuously evolve into larger crystals(Figure 1b and Figure S2, Supporting Information). However,at low nucleation density, crystals grow in random directions.Second, a steady contact line receding is needed. A dryingdroplet on a substrate typically will slide to a corner or edge,usually due to a slight tilt of the substrate. This sliding disruptsthe steady receding of the droplet, resulting in uncontrolledalignment (Figure S3, Supporting Information). In order toavoid sliding, we placed a small piece of Si wafer (which wetermed a pinner) at the center of the droplet, leading to asteady receding contact line (Figure 1a). We notice that Takeyagroup also used a piece of solid to sustain a inclined solutionfilm and achieved oriented organic crystals.41
During the DPC process, the shape, size, and location of thedroplet are determined by those of the pinner, which gives theDPC method several remarkable advantages. First, DPC iseasily scalable. The pinners can be patterned over a large areawith a controlled density. We scaled the processed area up to a100 mm wafer area (Figures 1c and 3). Around 50% of thewafer surface was covered by aligned crystals. This area fractionwill further increase if we decrease the size of the pinners. Weenvision that an even larger processed area should beachievable. Second, DPC can be used to define the location
Figure 1. Schematic representations of the DPC method. (a) An organic semiconductor droplet pinned by a silicon wafer. As the solvent evaporatesslowly, the crystals of the organic semiconductors nucleate near the contact line of the droplet. Subsequently, the nuclei grow along the recedingdirection (toward the center) of the droplet. (b) A magnified view of a white-marked area in (a), highlighting the contact line where a highnucleation density (right side) leads to unidirectional crystallization along the receding direction of the droplet, while a low nucleation density (leftside) results in nondirectional crystallization. (c) DPC can be scaled up by using multiple pinners with larger sizes. Elongation of the pinner leads tounidirectional parallel alignment of the crystals.